General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 8 - 8.01 g/cm³ Show Material materials with Density of 8 - 8.01 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | -100.0 °C | 206 GPa Show Material materials with Elastic modulus of 206 GPa |

20.0 °C | 196 - 200 GPa Show Material materials with Elastic modulus of 196 - 200 GPa | |

100.0 °C | 190 - 194 GPa Show Material materials with Elastic modulus of 190 - 194 GPa | |

200.0 °C | 182 - 186 GPa Show Material materials with Elastic modulus of 182 - 186 GPa | |

300.0 °C | 174 - 179 GPa Show Material materials with Elastic modulus of 174 - 179 GPa | |

400.0 °C | 166 - 172 GPa Show Material materials with Elastic modulus of 166 - 172 GPa | |

500.0 °C | 158 - 165 GPa Show Material materials with Elastic modulus of 158 - 165 GPa | |

600.0 °C | 150 GPa Show Material materials with Elastic modulus of 150 GPa | |

700.0 °C | 142 GPa Show Material materials with Elastic modulus of 142 GPa | |

800.0 °C | 134 GPa Show Material materials with Elastic modulus of 134 GPa | |

Elongation | 20.0 °C | 35 % Show Material materials with Elongation of 35 % |

Elongation, transverse | 20.0 °C | 30 % Show Material materials with Elongation, transverse of 30 % |

Poisson's ratio | 20.0 °C | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] |

Shear modulus | 20.0 °C | 77.3 GPa Show Material materials with Shear modulus of 77.3 GPa |

Tensile strength | 20.0 °C | 580 - 800 MPa Show Material materials with Tensile strength of 580 - 800 MPa |

Tensile strength, transverse | 20.0 °C | 580 - 800 MPa Show Material materials with Tensile strength, transverse of 580 - 800 MPa |

Yield strength Rp0.2 | 20.0 °C | 295 MPa Show Material materials with Yield strength Rp0.2 of 295 MPa |

50.0 °C | 255 MPa Show Material materials with Yield strength Rp0.2 of 255 MPa | |

100.0 °C | 215 MPa Show Material materials with Yield strength Rp0.2 of 215 MPa | |

150.0 °C | 195 MPa Show Material materials with Yield strength Rp0.2 of 195 MPa | |

200.0 °C | 175 MPa Show Material materials with Yield strength Rp0.2 of 175 MPa | |

250.0 °C | 165 MPa Show Material materials with Yield strength Rp0.2 of 165 MPa | |

300.0 °C | 155 MPa Show Material materials with Yield strength Rp0.2 of 155 MPa | |

350.0 °C | 150 MPa Show Material materials with Yield strength Rp0.2 of 150 MPa | |

400.0 °C | 145 MPa Show Material materials with Yield strength Rp0.2 of 145 MPa | |

450.0 °C | 140 MPa Show Material materials with Yield strength Rp0.2 of 140 MPa | |

500.0 °C | 138 MPa Show Material materials with Yield strength Rp0.2 of 138 MPa | |

550.0 °C | 136 MPa Show Material materials with Yield strength Rp0.2 of 136 MPa | |

Unlock all property charts | ||

Yield strength Rp0.2, transverse | 20.0 °C | 295 MPa Show Material materials with Yield strength Rp0.2, transverse of 295 MPa |

Yield strength Rp1.0 | 20.0 °C | 330 MPa Show Material materials with Yield strength Rp1.0 of 330 MPa |

50.0 °C | 290 MPa Show Material materials with Yield strength Rp1.0 of 290 MPa | |

100.0 °C | 245 MPa Show Material materials with Yield strength Rp1.0 of 245 MPa | |

150.0 °C | 225 MPa Show Material materials with Yield strength Rp1.0 of 225 MPa | |

200.0 °C | 205 MPa Show Material materials with Yield strength Rp1.0 of 205 MPa | |

250.0 °C | 195 MPa Show Material materials with Yield strength Rp1.0 of 195 MPa | |

300.0 °C | 185 MPa Show Material materials with Yield strength Rp1.0 of 185 MPa | |

350.0 °C | 180 MPa Show Material materials with Yield strength Rp1.0 of 180 MPa | |

400.0 °C | 175 MPa Show Material materials with Yield strength Rp1.0 of 175 MPa | |

450.0 °C | 170 MPa Show Material materials with Yield strength Rp1.0 of 170 MPa | |

500.0 °C | 168 MPa Show Material materials with Yield strength Rp1.0 of 168 MPa | |

550.0 °C | 166 MPa Show Material materials with Yield strength Rp1.0 of 166 MPa | |

Unlock all property charts |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 1/K | |

20.0 °C | 1.61E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.61E-5 1/K | ||

100.0 °C | 1.6E-5 - 1.67E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.6E-5 - 1.67E-5 1/K | ||

200.0 °C | 1.65E-5 - 1.72E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.65E-5 - 1.72E-5 1/K | ||

300.0 °C | 1.7E-5 - 1.77E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.7E-5 - 1.77E-5 1/K | ||

400.0 °C | 1.75E-5 - 1.81E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.75E-5 - 1.81E-5 1/K | ||

500.0 °C | 1.8E-5 - 1.84E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.8E-5 - 1.84E-5 1/K | ||

600.0 °C | 1.88E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.88E-5 1/K | ||

700.0 °C | 1.91E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.91E-5 1/K | ||

800.0 °C | 1.94E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.94E-5 1/K | ||

900.0 °C | 1.97E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.97E-5 1/K | ||

1000.0 °C | 2E-5 1/K Show Material materials with Coefficient of thermal expansion of 2E-5 1/K | ||

Unlock all property charts | |||

Melting point | 1230 - 1480 °C Show Material materials with Melting point of 1230 - 1480 °C | Typical for Austenitic Stainless Steel | |

Specific heat capacity | -100.0 °C | 440 J/(kg·K) Show Material materials with Specific heat capacity of 440 J/(kg·K) | |

20.0 °C | 472 - 500 J/(kg·K) Show Material materials with Specific heat capacity of 472 - 500 J/(kg·K) | ||

100.0 °C | 487 J/(kg·K) Show Material materials with Specific heat capacity of 487 J/(kg·K) | ||

200.0 °C | 503 J/(kg·K) Show Material materials with Specific heat capacity of 503 J/(kg·K) | ||

300.0 °C | 512 J/(kg·K) Show Material materials with Specific heat capacity of 512 J/(kg·K) | ||

400.0 °C | 520 J/(kg·K) Show Material materials with Specific heat capacity of 520 J/(kg·K) | ||

500.0 °C | 530 J/(kg·K) Show Material materials with Specific heat capacity of 530 J/(kg·K) | ||

600.0 °C | 541 J/(kg·K) Show Material materials with Specific heat capacity of 541 J/(kg·K) | ||

700.0 °C | 551 J/(kg·K) Show Material materials with Specific heat capacity of 551 J/(kg·K) | ||

800.0 °C | 559 J/(kg·K) Show Material materials with Specific heat capacity of 559 J/(kg·K) | ||

900.0 °C | 565 J/(kg·K) Show Material materials with Specific heat capacity of 565 J/(kg·K) | ||

1000.0 °C | 571 J/(kg·K) Show Material materials with Specific heat capacity of 571 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 13.5 - 15 W/(m·K) Show Material materials with Thermal conductivity of 13.5 - 15 W/(m·K) | |

100.0 °C | 14.9 W/(m·K) Show Material materials with Thermal conductivity of 14.9 W/(m·K) | ||

200.0 °C | 16.7 W/(m·K) Show Material materials with Thermal conductivity of 16.7 W/(m·K) | ||

300.0 °C | 18.3 W/(m·K) Show Material materials with Thermal conductivity of 18.3 W/(m·K) | ||

400.0 °C | 19.8 W/(m·K) Show Material materials with Thermal conductivity of 19.8 W/(m·K) | ||

500.0 °C | 21.3 W/(m·K) Show Material materials with Thermal conductivity of 21.3 W/(m·K) | ||

600.0 °C | 22.7 W/(m·K) Show Material materials with Thermal conductivity of 22.7 W/(m·K) | ||

700.0 °C | 24.2 W/(m·K) Show Material materials with Thermal conductivity of 24.2 W/(m·K) | ||

800.0 °C | 25.6 W/(m·K) Show Material materials with Thermal conductivity of 25.6 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 3.6 mm²/s Show Material materials with Thermal diffusivity of 3.6 mm²/s | |

100.0 °C | 3.7 mm²/s Show Material materials with Thermal diffusivity of 3.7 mm²/s | ||

200.0 °C | 4 mm²/s Show Material materials with Thermal diffusivity of 4 mm²/s | ||

300.0 °C | 4.4 mm²/s Show Material materials with Thermal diffusivity of 4.4 mm²/s | ||

400.0 °C | 4.6 mm²/s Show Material materials with Thermal diffusivity of 4.6 mm²/s | ||

500.0 °C | 4.7 mm²/s Show Material materials with Thermal diffusivity of 4.7 mm²/s | ||

600.0 °C | 4.9 mm²/s Show Material materials with Thermal diffusivity of 4.9 mm²/s | ||

700.0 °C | 5.2 mm²/s Show Material materials with Thermal diffusivity of 5.2 mm²/s | ||

800.0 °C | 5.5 mm²/s Show Material materials with Thermal diffusivity of 5.5 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 7.5E-7 - 7.75E-7 Ω·m Show Material materials with Electrical resistivity of 7.5E-7 - 7.75E-7 Ω·m |

100.0 °C | 8.42E-7 Ω·m Show Material materials with Electrical resistivity of 8.42E-7 Ω·m | |

200.0 °C | 9.04E-7 Ω·m Show Material materials with Electrical resistivity of 9.04E-7 Ω·m | |

300.0 °C | 9.62E-7 Ω·m Show Material materials with Electrical resistivity of 9.62E-7 Ω·m | |

400.0 °C | 1.01E-6 Ω·m Show Material materials with Electrical resistivity of 1.01E-6 Ω·m | |

500.0 °C | 1.06E-6 Ω·m Show Material materials with Electrical resistivity of 1.06E-6 Ω·m | |

600.0 °C | 1.1E-6 Ω·m Show Material materials with Electrical resistivity of 1.1E-6 Ω·m | |

700.0 °C | 1.13E-6 Ω·m Show Material materials with Electrical resistivity of 1.13E-6 Ω·m | |

800.0 °C | 1.16E-6 Ω·m Show Material materials with Electrical resistivity of 1.16E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.03 % Show Material materials with Carbon of 0.03 % |

Chromium | 16.5 - 18.5 % Show Material materials with Chromium of 16.5 - 18.5 % |

Manganese | 2 % Show Material materials with Manganese of 2 % |

Molybdenum | 2.5 - 3 % Show Material materials with Molybdenum of 2.5 - 3 % |

Nickel | 11 - 14 % Show Material materials with Nickel of 11 - 14 % |

Nitrogen | 0.12 - 0.22 % Show Material materials with Nitrogen of 0.12 - 0.22 % |

Phosphorus | 0.05 % Show Material materials with Phosphorus of 0.05 % |

Silicon | 1 % Show Material materials with Silicon of 1 % |

Sulfur | 0.015 % Show Material materials with Sulfur of 0.015 % |